Production of bioabsorbible nanoparticles of polycaprolactone by using a tubular recirculating system • Gabriel Colmenares-Roldán ac, Liliana Agudelo-Gómez a,c, Rodolfo Pinal b &, Lina Hoyos- Palacio a,c a
Grupo de Investigación en Biología de Sistemas, Escuela de Ciencias de la Salud, Universidad Pontificia Bolivariana, Medellín, Colombia, [email protected]
b Department of Industrial & Physical Pharmacy, College of Pharmacy, Purdue University, Indiana, USA, [email protected]
c Grupo de Investigación en Nanotecnología y Materiales, Nanomat, Medellín, Colombia, [email protected]
Received: January 30th, 2017. Received in revised form: October 13st, 2017. Accepted: December 15th, 2017.
Abstract Encapsulation and controlled release of substances using polymeric nanoparticles require that these have a high reproducibility, homogeneity, and control over their properties, especially when they are to be used in medical, pharmaceutical or nutritional applications among others. This work shows a high productivity system to synthesize nanoparticles in an easy, fast and controlled way. This study shows the effect of molecular weight of the polymer, the type of surfactant and the relationship between the volumes of the aqueous and the organic phases. It was found that the first two variables have a statistically significant effect on the diameter of the nanoparticles while the relationship between the volume of the aqueous phase and the organic phase does not significantly affect the diameter of the nanoparticles. Additionally, it was found that none of the three variables significantly affects the polydispersity index (PI) of the nanoparticles. Keywords: nanoparticles; polycaprolactone; nanoprecipitation; encapsulation; delivery
Producción de nanopartículas bioabsorbibles de policaprolactona empleando un sistema de recirculación tubular Resumen La encapsulación y la liberación controlada de sustancias que utilizan nanopartículas poliméricas requieren que estas tengan una alta reproducibilidad, homogeneidad y control sobre sus propiedades, especialmente cuando se van a utilizar en aplicaciones médicas, farmacéuticas o nutricionales entre otras. Este trabajo muestra un sistema de alta productividad para sintetizar nanopartículas poliméricas de una forma fácil, rápida y de manera controlada. Este estudio muestra el efecto del peso molecular del polímero, el tipo de tensioactivo y la relación entre los volúmenes de las fases acuosa y orgánica. Se encontró que las dos primeras variables tienen un efecto estadísticamente significativo sobre el diámetro de las nanopartículas, mientras que la relación entre el volumen de la fase acuosa y la fase orgánica no afecta significativamente el diámetro de las nanopartículas. Además, se encontró que ninguna de las tres variables afecta significativamente el índice de polidispersidad de las nanopartículas. Palabras clave: nanopartículas; policaprolactona; nanoprecipitación; encapsulación; liberación.
1. Introduction The appropriate design of encapsulation systems and controlled release systems for multiple applications in the pharmaceutical, nutrition, agricultural, textile, paints and personal care, among others, can guarantee the delivery and preservation in
the short, medium and long-term of different substances [1,2]. The use of nanoparticles, specifically polymeric nanoparticles in controlled release, is a subject of increasing interest of study [3-5]. Nanoparticles of biodegradable polymers are considered important for drug delivery systems since they are very stable, easily adapt to industrial manufacturing processes over other types of nanoparticles and can be modified at their surfaces to modulate
How to cite: Colmenares-Roldan, G.J., Agudelo-Gomez, L.M., Pinal, R. and Hoyos-Palacio, L.M., Production of bioabsorbible nanoparticles of polycaprolactone by using a tubular recirculating system. DYNA, 85(204), pp. 277-282, March, 2018.
© The author; licensee Universidad Nacional de Colombia. Revista DYNA, 85(204), pp. 277-282, March, 2018, ISSN 0012-7353 DOI: http://dx.doi.org/10.15446/dyna.v85n204.62292
Colmenares-Roldan et al / Revista DYNA, 85(204), pp. 277-282, March, 2018.
their properties [1,6-9]. Additionally, polymeric nanoparticles can be engineered to control the rate of release of drugs as well as to control their release at a specific site in the body (9). The modulation of their characteristics is achieved through the properties of the polymer and the chemical composition of the surface of the nanoparticles [9,10]. To date, conventional bulk synthesis methods for the production of polymer nanoparticles have been studied, such as nanoprecipitation, emulsion-diffusion, emulsion-coacervation, double emulsion, polymer coating, supercritical fluids and layer by layer deposition, among others [11-13]. Despite advances in each of these methodologies, the scientific community continues to face a significant challenge, namely, to guarantee the properties and reproducibility of the nanoparticles as well as to scale these systems for use in clinical trials [14,15]. The main concern in conventional bulk synthesis methods is the heterogeneous mixing. This usually takes too much time and requires a lot of energy, which results in an expensive process and produces larger and polydisperse particles . Recent studies, show that microfluidic platform can enhance the controllability and reproducibility of synthesized nanoparticles compared to the conventional bulk synthesis method, because the microfluidic platform can offer precisely controlled reaction environments like rapid mixing of reagents, control of temperature, and precise spatiotemporal manipulation of reactions that are difficult, if not impossible, in larger reactors. However, the productivity of microfluidic systems is lower than that of batch reactors due to low flow rates, which can limit the application of nanoparticles synthesized by microfluidic systems [17-20]. This work introduces a system for synthesizing polymeric nanoparticles with high productivity. The approach can easily control the characteristics of the nanoparticles obtained and does not require specialized equipment. Additionally, the system is quite flexible and can produce small amounts of nanoparticles or it can be readily adjusted to produce large amounts. The system is based on a continuous tubular reactor that initially recirculates the aqueous phase. The organic phase is injected into the aqueous stream. The turbulence of the system in the pipe section leads to the immediate formation of nanoparticles by the phenomenon of nanoprecipitation. The present work evaluated the flow relationship between the two currents, the molecular weight of the polymer and the influence of the surfactants in the system.
of the tubular reactor used was VMQ (Vinyl Methyl-Quality) solvent-resistant silicone tubing, used in the organic phase for this study. It is recommended that materials complying with USP Class VI specifications be used. The injection of the organic phase can be modulated by changing the injection needle (18G, 20G, 21G, 22G, 23G, 25G, 27G, 29G, 30G, 31G) and modulating the injection rate, thereby controlling the particle size distribution of the nanoparticles. For this work, the 30G needle was used. Peristaltic pumps were used to control flow rates in this system. In this system, the flow rates of the organic phase and the recirculation stream can be adjusted, varying the turbulence and the flow ratio between the two, thus controlling the size and polydispersity of the nanoparticles obtained. The recirculation system is described in Fig. 1 and the process of preparation of the nanoparticles step by step in the Fig. 2.
Figure 1. Description of the recirculating system Source: Authors
2. Materials Polycaprolactone (PCL) Mw=14,000, 45,000 and 80,000 g⋅mol-1, Acetone and surfactants (Pluronic F-127, Poloxamer 188 and Tween 80) were purchased from Sigma Aldrich 3. Methods 3.1. Recirculating system The recirculation system is based on a continuous tubular reactor with adjustable length and tubular diameters, depending on the performance requirements. The length of the system can be varied from 30cm to 15m and the internal diameter of the reactor from 0.79mm to 38mm. For this work, the diameter of the reactor used was 3.175mm. The material
Figure 2. The process of preparation of the nanoparticles step by step using the recirculation system. Source: Authors
Colmenares-Roldan et al / Revista DYNA, 85(204), pp. 277-282, March, 2018.
3.2. Preparation of the nanoparticles
3.5. Size and size distribution
To prepare the nanoparticles, it was necessary to use two phases. First, the organic phase was prepared to contain the polymer, the solvent and the active compound to encapsulate. Subsequently, the aqueous phase was prepared with deionized water and one or more surfactants. Is possible to use some additives both phases in order to modify the properties of the final nanoparticles. Fig. 2 shows the process used to prepare the polymeric nanoparticles using the recirculating system from the preparation of the precursor solutions, the operation of the recirculation system, the recovery of the nanoparticles and the characterization of the nanoparticles.
The nanoparticle size and polydispersity index (PI) were evaluated by dynamic light scattering (DLS) using a Malvern Zetasizer (Nano ZS, Malvern Instruments). All measurements were carried out at 25 °C using a refractive index of 1.44 and material absorption of 0.001.
3.3. Design of experiments
In previous work carried out by the research group, it was found that the diameter of the polymer nanoparticles strongly depends on the turbulence generated in the recirculation system. For this reason, the flow rate of the recirculation system was set at 162mL⋅min-1 for a Reynolds number of Re=1,249 . The statistical analysis of this work was carried out using the software Statgraphics Centurion XV. For this design of experiments, three variables (molecular weight of the polymer, type of surfactant and ratio between the aqueous phase and the organic phase) were used, each with three level as shown in Fig. 3, for a total of 27 trials. The concentration of polymers in the organic phases used in this work was 4mg⋅mL-1 and the concentration of the surfactants in the aqueous phases was 0.25% w/v according to previous tests . All assays were performed with 20 mL of the organic phase and the volume of the aqueous phase was adjusted according to the ratio of each assay (40mL, 100mL, and 200mL).
4.1. Statistical analysis of DLS results
3.4. Morphology Transmission electron microscopy (TEM) with TEM microscope (FEI Tecnai T20) was used to study nanoparticle morphology. A droplet of the sample was mixed with a contrasting agent (1% phosphotungstic acid, pH 7.0 adjusted with 1M KOH solution) was placed on a carbon grid. The grid was pushed onto the surface of the droplet in order to create a film over the grid. The prepared sample was then placed in the TEM after 5 min for analysis.
3.6. Statistical analysis Statistical analysis of the particle size was performed applying multifactorial variance (ANOVA) using the program Statgraphics Centurion XV. Differences were considered to be significant at a level of p < 0.05.
With the experimental design employed, it was possible to study the effect of the three design variables on the recirculation system and their effect on the diameter and polydispersity of the nanoparticles. The analysis of variance for the average diameter (Zave) of the nanoparticles revealed that the molecular weight of the polymer (p = 0.0247) and the surfactant type (p = 0.0012) have both p